172 



JAMES NANGLE. 



TABULATED EESULTS- 



— Continued. 





Botanical Name. 



Breaking 

 Load, in 



Modulus of 

 rupture in 



Modulus of 

 elasticity in 



Eate of 

 Load in 



(Common Name.) 



Pounds. 



lbs. per 

 sq. inch. 



lbs. per 

 square inch. 



lbs. per 

 minute. 



1. Clear Pine... 



3,346 



6,570 







2. do 



4,120 



8,158 







3. do 



3,725 



7,018 





... 



1. American Redwood 



5,100 



10,200 



1,565,217 



510 



2. do 



3,500 



7,010 



1,524,705 



350 



3. do 



5,130 



10,613 



1,690,217 



570 



1. Pitch Pine 



8,000 



15,686 



2,717,825 



296 



2. do 



7,600 



15,000 



2,061,384 



760 



3. do 



7,000 



14,000 



2,273,684 



636 



1. Japanese Pine 



4,000 



9,424 



1,325,454 



800 



2. do 



3,775 



9,208 



1,035,266 



377 



3. do 



3,300 



9,166 



1,500,000 



412 



1. Red Baltic Pine ... 



5.100 



11,149 



2,087,584 



463 



2. do 



5,600 



12,573 



2,168,029 



560 



3. do 



5,200 



11,675 



2,943,596 



520 



1. White Baltic Pine 



2.510 



6,435 



1,714,285 



358 



2. do. 



2,555 



6,328 



1,749,600 



425 



3. do. 



3,745 



9,276 



1,682,307 



416 



1. Pacific Pine 



3,000 



6,000 



1,440,000 



500 



2. do. 



3,200 



6,400 



1,183,561 



640 



3. do. 



3,500 



7,000 



1,270,588 700 



V. Vernacular 



American Ash 

 American Hickory- 

 American Redwood 

 Ash (American) 

 Baltic Pine (Red) 

 Baltic Pine (White) 

 Beech (Red) 

 Black or Cypress Pine 

 Blackbutt 



Black Myrtle (Grey Plum 

 Blackwood 

 Blue Gum (Sydney) 

 Brown Pine 

 Burmah Teak 



Names of Timbers Tested. 



Messmate 

 Mountain Ash 

 Murray River Red Gum 

 Myrtle (Tasmanian) 

 New England Peppermint 

 Negor Head Beech 

 Oregon 

 Pacific Pine 



Peppermint (New England) 

 ) Pine (Clear) 



Pitch Pine 

 Queensland Maple 

 Red Wood (American) 

 Red Beech 



